# Fracture

﻿
Fracture
v · d · e Materials failure modes

A fracture is the (local) separation of an object or material into two, or more, pieces under the action of stress.

The word fracture is often applied to bones of living creatures (that is, a bone fracture), or to crystals or crystalline materials, such as gemstones or metal. Sometimes, in crystalline materials, individual crystals fracture without the body actually separating into two or more pieces. Depending on the substance which is fractured, a fracture reduces strength (most substances) or inhibits transmission of light (optical crystals).

A detailed understanding of how fracture occurs in materials may be assisted by the study of fracture mechanics.

## Fracture strength

Stress vs. strain curve typical of aluminum
1. Ultimate tensile strength
2. Yield strength
3. Proportional limit stress
4. Fracture
5. Offset strain (typically 0.2%)

Fracture strength, also known as breaking strength, is the stress at which a specimen fails via fracture.[1] This is usually determined for a given specimen by a tensile test, which charts the stress-strain curve (see image). The final recorded point is the fracture strength.

Ductile materials have a fracture strength lower than the ultimate tensile strength (UTS), whereas in brittle materials the fracture strength is equivalent to the UTS.[1] If a ductile material reaches its ultimate tensile strength in a load-controlled situation,[Note 1] it will continue to deform, with no additional load application, until it ruptures. However, if the loading is displacement-controlled,[Note 2] the deformation of the material may relieve the load, preventing rupture.

If the stress-strain curve is plotted in terms of true stress and true strain the curve will always slope upwards and never reverse, as true stress is corrected for the decrease in cross-sectional area. The true stress on the material at the time of rupture is known as the breaking strength. This is the maximum stress on the true stress-strain curve, given by point 3 on curve B.

## Types

### Brittle fracture

Brittle fracture in glass.
Fracture of an Aluminum Crank Arm. Bright: Brittle fracture. Dark: Fatigue fracture.

In brittle fracture, no apparent plastic deformation takes place before fracture. In brittle crystalline materials, fracture can occur by cleavage as the result of tensile stress acting normal to crystallographic planes with low bonding (cleavage planes). In amorphous solids, by contrast, the lack of a crystalline structure results in a conchoidal fracture, with cracks proceeding normal to the applied tension.

The theoretical strength of a crystalline material is (roughly)

$\sigma_\mathrm{theoretical} = \sqrt{ \frac{E \gamma}{r_o} }$

where: -

E is the Young's modulus of the material,
γ is the surface energy, and
ro is the equilibrium distance between atomic centers.

On the other hand, a crack introduces a stress concentration modeled by

$\sigma_\mathrm{elliptical\ crack} = \sigma_\mathrm{applied}\left(1 + 2 \sqrt{ \frac{a}{\rho}}\right) = 2 \sigma_\mathrm{applied} \sqrt{\frac{a}{\rho}}$ (For sharp cracks)

where: -

a is half the length of the crack, and
ρ is the radius of curvature at the crack tip.

Putting these two equations together, we get

$\sigma_\mathrm{fracture} = \sqrt{ \frac{E \gamma \rho}{4 a r_o}}.$

Looking closely, we can see that sharp cracks (small ρ) and large defects (large a) both lower the fracture strength of the material.

Recently, scientists have discovered supersonic fracture, the phenomenon of crack motion faster than the speed of sound in a material.[citation needed] This phenomenon was recently also verified by experiment of fracture in rubber-like materials.

### Ductile fracture

Ductile failure of a specimen strained axially.
Schematic representation of the steps in ductile fracture (in pure tension).

In ductile fracture, extensive plastic deformation (necking) takes place before fracture. The terms rupture or ductile rupture describe the ultimate failure of tough ductile materials loaded in tension. Rather than cracking, the material "pulls apart," generally leaving a rough surface. In this case there is slow propagation and an absorption of a large amount energy before fracture.[citation needed]

Many ductile metals, especially materials with high purity, can sustain very large deformation of 50–100% or more strain before fracture under favorable loading condition and environmental condition. The strain at which the fracture happens is controlled by the purity of the materials. At room temperature, pure iron can undergo deformation up to 100% strain before breaking, while cast iron or high-carbon steels can barely sustain 3% of strain.[citation needed]

Because ductile rupture involves a high degree of plastic deformation, the fracture behavior of a propagating crack as modeled above changes fundamentally. Some of the energy from stress concentrations at the crack tips is dissipated by plastic deformation before the crack actually propagates.

The basic steps are: void formation, void coalescence (also known as crack formation), crack propagation, and failure, often resulting in a cup-and-cone shaped failure surface.

## Crack separation modes

The three fracture modes.

There are three ways of applying a force to enable a crack to propagate:

• Mode I crack – Opening mode (a tensile stress normal to the plane of the crack)
• Mode II crack – Sliding mode (a shear stress acting parallel to the plane of the crack and perpendicular to the crack front)
• Mode III crack – Tearing mode (a shear stress acting parallel to the plane of the crack and parallel to the crack front)

Crack initiation and propagation accompany fracture. The manner through which the crack propagates through the material gives great insight into the mode of fracture. In ductile materials (ductile fracture), the crack moves slowly and is accompanied by a large amount of plastic deformation. The crack will usually not extend unless an increased stress is applied. On the other hand, in dealing with brittle fracture, cracks spread very rapidly with little or no plastic deformation. The cracks that propagate in a brittle material will continue to grow and increase in magnitude once they are initiated. Another important mannerism of crack propagation is the way in which the advancing crack travels through the material. A crack that passes through the grains within the material is undergoing transgranular fracture. However, a crack that propagates along the grain boundaries is termed an intergranular fracture.

## Notes

1. ^ A simple load-controlled tensile situation would be to support a specimen from above, and hang a weight from the bottom end. The load on the specimen is then independent of its deformation.
2. ^ A simple displacement-controlled tensile situation would be to attach a very stiff jack to the ends of a specimen. As the jack extends, it controls the displacement of the specimen; the load on the specimen is dependent on the deformation.

## References

1. ^ a b Degarmo, E. Paul; Black, J T.; Kohser, Ronald A. (2003), Materials and Processes in Manufacturing (9th ed.), Wiley, p. 32, ISBN 0-471-65653-4.

• Dieter, G. E. (1988) Mechanical Metallurgy ISBN 0-07-100406-8
• A. Garcimartin, A. Guarino, L. Bellon and S. Cilberto (1997) " Statistical Properties of Fracture Precursors ". Physical Review Letters, 79, 3202 (1997)
• Callister, Jr., William D. (2002) Materials Science and Engineering: An Introduction. ISBN 0-471-13576-3
• Peter Rhys Lewis, Colin Gagg, Ken Reynolds, CRC Press (2004), Forensic Materials Engineering: Case Studies.

Wikimedia Foundation. 2010.

Synonyms:

### Look at other dictionaries:

• fracture — [ fraktyr ] n. f. • 1391; fraiture fin XIIe; lat. fractura, de frangere → fraction 1 ♦ Vx Rupture avec violence, avec effort. ⇒ bris. État de ce qui est fracturé, rompu. ⇒ cassure. Mod. Géol. Cassure de l écorce terrestre. ⇒ 2. faille; coupure.… …   Encyclopédie Universelle

• Fracture — Frac ture (?; 135), n. [L. fractura, fr. frangere, fractum, to break: cf. F. fracture. See {Fraction}.] 1. The act of breaking or snapping asunder; rupture; breach. [1913 Webster] 2. (Surg.) The breaking of a bone. [1913 Webster] 3. (Min.) The… …   The Collaborative International Dictionary of English

• Fracture — Разработчики Day 1 Studios …   Википедия

• Fracture — Frac ture (?; 135), v. t. [imp. & p. p. {Fractured} (#; 135); p. pr. & vb. n.. {Fracturing}.] [Cf. F. fracturer.] To cause a fracture or fractures in; to break; to burst asunder; to crack; to separate the continuous parts of; as, to fracture a… …   The Collaborative International Dictionary of English

• Fracture — bezeichnet: den US amerikanischen Thriller Das perfekte Verbrechen (Fracture) aus dem Jahr 2007 den Titel des neuseeländischen Films Fracture (2004) aus dem Jahr 2004 ein Shooter Videospiel Fracture (Spiel) von Lucas Arts Diese …   Deutsch Wikipedia

• fracture — Fracture. s. f. Rupture avec effort. Fracture de portes. il y a fracture à l os …   Dictionnaire de l'Académie française

• fracture — [frak′chər] n. [ME < OFr < L fractura, a breaking, breach, cleft < pp. of frangere, BREAK] 1. a breaking or being broken 2. a break, crack, or split 3. a break in a body part, esp. in a bone, or a tear in a cartilage: see COMPOUND… …   English World dictionary

• fracturé — fracturé, ée (fra ktu ré, rée) part. passé de fracturer. Un membre fracturé …   Dictionnaire de la Langue Française d'Émile Littré

• fracture — (n.) early 15c., a breaking of a bone, from M.Fr. fracture (14c.), from L. fractura a breach, break, cleft, from fractus, pp. of frangere to break (see FRACTION (Cf. fraction)). The verb is first recorded 1610s (implied in fractured). Related:… …   Etymology dictionary

• Fracture — Fracture. См. Разрушение. (Источник: «Металлы и сплавы. Справочник.» Под редакцией Ю.П. Солнцева; НПО Профессионал , НПО Мир и семья ; Санкт Петербург, 2003 г.) …   Словарь металлургических терминов

• fracture — index hiatus, rend, rift (gap), split (noun), split (verb) Burton s Legal Thesaurus. William C. Burton. 2006 …   Law dictionary